1 ASTM A234/A234M-10 . Standard Specification for Pipes Fittings of Wrought Carbon Steel and Alloy Steel for Moderate and High Temperature Service 1. Scope :- this Specification covers wrought carbon steel and alloy steel fittings of seamless and welded construction covered by the latest revision of ASME , , MSS-SP- 79 , MSS-SP 83 , MSS-SP-95 , and MSS-SP-97 . These fittings are for use in pressure piping and in pressure vessel fabrication for service at moderate and elevated temperatures. Fittings differing from these ASME and MSS standards shall be furnished in according with Supplementary Requirement S58 of Specification A960/A960M. optional supplementary requirements are provided for fitting where a greater degree of examination is desired.
2 When desired , one of more of these supplementary requirements may be specified in the order. This Specification does not cover cash welding fittings or fittings machined from castings. Cast steel welding fittings are governed by Specification A216/A216M and A217/A217M . This Specification is expressed in both inch-pound units and in SI units. However , unless the order specifies the applicable M Specification designation (SI. units) , the material shall be furnished to inch-pound units . The values stated in either SI units or inch-pound units are to be regarded separately as Standard . Within the text , the Si units are shown in brackets . the value stated in each system may not be exact equivalents ; therefore ; each system shall be used independently of the order.
3 Combining values from the two systems may result in non-conformance with the Standard . 2. Referenced Documents :- In addition to those reference documents listed in Specification A960/A960M , the following list of standards apply to this Specification . ASTM Standards :- A216/A216N Specification for Steel castings , Carbon , Suitable for Fusion Welding , for High-Temperature Service A217/A217M Specification for steel Castings , Martensitic Stainless and Alloy , for Pressure-Containing Parts , Suitable for High-Temperature Service A960/A960M Specification for Common requirements for Wrought steel Piping fittings Direct No. :- +91-022-43431307 Fax No. :- +91-022-23894511 Email :- Board No. :- +91-022-43431313 Website :- Page |1.
4 ASTM A234/A234M-10 . ASME standards :- Steel Butt-Welding fittings Forged Steel Fittings , Socket Welding and Threaded ASME Boiler and Pressure Vessel Cde: Section V Nondestructive Examination Section VIII , Division 1 , pressure Vessels Section IX Welding Qualifications MSS Standards :- MSS-SP-25 Standard Marking System for Values , Fittings , Flanges , and Unions MSS-SP-79 Socket Welding Reducer Inserts MSs-SP-83 Steel Pipe Unions , Socket-Welding and Threaded MSS-SP-95 Swage (d) Nipples and Bull Plugs MSS-SP-97 Integrally Reinforced Forged Branch outlet Fittings-Socket Welding , Threaded and Buttwelding Ends ASNT Standard :- SNT-TC-1A Recommended Practice for Nondestrutive testing Personal Qualification and Certification AWS Specifications :- Specification for low Alloy Steel Electrodes for Shielded Metal Arc Welding Specification for Low Alloy Steel electrodes and Fluxes for Submerged Arc welding Specification for Low-Alloy Steel Electrodes for Gas Shielded Arc Welding Low-Alloy Steel Electrodes for Flux Cored Arc Welding 3.
5 Ordering Information See Specification A960/A960M. 4. General requirements :- Product furnished to this Specification shall conform to the requirements of Specification A960/A960M , including any the supplementary requirements that are including in the purchase order . Failure to comply with this Specification . In case of a conflict between the requirement of this Specification and Specification A960/A960M , this Specification shall prevail. Direct No. :- +91-022-43431307 Fax No. :- +91-022-23894511 Email :- Board No. :- +91-022-43431313 Website :- Page |2. ASTM A234/A234M-10 . TABLE 1 Chemical Requirements Composition , %. Grade and Marking carbon Manga- Phosp- Sulfur, Silicon Chor- Moly- Nickal Cop- Others Symbol neses horus, max mium bdenum per max WPB max Vanadium max min max max max max WPC max Vanadium max min max max max max WP1.
6 Max WP12 .. CL1,WP12 max CL2. WP11 CL1 .. WP11 CL2, .. WP11 CL3 WP22 CL1 , .. WP22 CL3 max WP5 CL1, .. WP5 CL3 max max WP9 CL1, .. WP9 CL3 max max WPR .. max WP91 .. Vanadium max Columbium Nitrogen Aluminium max . Titanium max . Zirconium max . WP911 .. Vanadium max Columbium Nitrogen Aluminium Direct No. :- +91-022-43431307 Fax No. :- +91-022-23894511 Email :- Board No. :- +91-022-43431313 Website :- Page |3. ASTM A234/A234M-10 . max . Boron Tungsten Titanium max . Zirconium max . TABLE 2 Tensile Requirements WP11 WP11. WPC , CL1 , CL3 , Grade and WPB WP11 WP1 WP22 WPR WP22 WP91 WP911 WP12. Marking Symbol CL2 , CL1, CL3 , CL1. WP12 WP5 WP5 CL3. CL2 CL1 , , WP9 WP9 CL3. CL1. Tensile strength , 60-90 70-95 55-80 60-85 63-88 75-100 85-110 90-120 60-85.
7 Range [415- [485-655] [380- [415- [435- [520- [585- [620- [415- Ksi [MPa] 655] 585] 585] 605] 690] 760] 840] 585]. Yield strength, Min,ksi,[MPa] 35 40 30 30 46 45 60 64 32. ( offset or         . extension- Under-load). 7. Heat Treatment :- Heat Treatment Procedures fittings , after forming at an elevated temperature below the critical range under suitable conditions to prevent injurious defects caused by too rapid cooling , but in no case more rapidly than the cooling rate in still air . Heat treatment temperature specified are metal (part) temperatures . Heat- treatment fittings shall be treated according to paragraph 7 in Specification A960/A960M.
8 WPB , WPC , and WPR Fittings : Direct No. :- +91-022-43431307 Fax No. :- +91-022-23894511 Email :- Board No. :- +91-022-43431313 Website :- Page |4. ASTM A234/A234M-10 . Hot-formed WPB , WPC , and WPR fittings upon which the final forming operation is completed at a temperature above 1150 F [620 C ] and below 1800 F. [980 C] need not be heat treatment provided they are cooled in still air . Hot-formed or forged WPB , WPC , and WPR fitting finished at temperature in excess of 1800 F [980 C] shall subsequently be annealed , normalised , or normalized and tempered . Hot-forged fittings NPS 4 or smaller need not be heat treated . WPB , WPC , and WPR fittings over NPS 12 , produced by locally heating a portion of the fitting stock to any temperature for forming , shall be subsequently annealed , normalized , or normalized and tempered.
9 Fittings such as elbows tees , header tees , reducers and lap joint stub ends with a carbon content less than , NPS 12 and under , shall not require heat treatment after forming a locally heated portion of the fitting . Cold-formed WPB , WPC , and WPR fittings upon which the final forming operation is completed at a temperature below 1150 F [620 C] , shall be normalized , or shell be stress relieved at 1100 at 1250 F [595 to 675 C] . WPB , WPC , and WPR fittings produced by fusion welding and having a normal wall thickness at the welded joint of in . [19 mm] or greater shall be post-weld heat treated at 1100 to 1250 F [595 to 675 C] , or in accordance with . At the option of the manufacture , WPB and WPC fittings produced by any of the method in Section 6 may be annealed , normalized , or normalized and tempered.
10 Fittings Other than WPB , WPC , and WPR : Fittings of Grades WP1 ,WP11 Class 1 , WP11 Class 2 , WP11 Class 3 , WP12. Class 1 , WP12 Class 2 , WP22 Class 1 , WP22 Class 3 , WP5 , and WP9 shall be finished in the full-annealed , isothermal annealed , or normalized and tempered condition . If normalized and tempered , the tempering temperature for WP11 Class 1 , WP11 Class 2 , WP11 Class3 , WP12 Class 1 , and WP12 Class 2 shall not be less than 1150 F [620 C] for Grades WP5 , WP9 , WP22 Class 1 , and WP22 Class 3 the tempering temperature shall not be less than 1250 F [675 C] . of Grades WP1 , WP12 , Class 1 , or WP12 heat treatment at 1200 F. [650 C] instead of the heat treatment specified in . Fittings in all thickness produced by fusion welding after heat treatment specified in shall be post-weld heat treated at a temperature not less than prescribed above for tempering except that Grade WP1 is required to be post-weld heat treated only when the normal wall thickness at the welded joint is in.